{'fraction_non_alphanumeric': 0.033816425120772944, 'fraction_numerical': 0.024154589371980676, 'mean_word_length': 5.0931372549019605, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Pyramid nano-voids in GaN and InGaN

High resolution transmission electron microscopy and aberration-corrected scanning transmission electron microscopy (STEM) reveal a new void defect in GaN, Si-doped GaN, and InGaN. The voids are pyramid shaped with symmetric hexagonal {0001} base facets and {10-11} side facets. The pyramid void has a closed or open core dislocation at the peak of the pyramid, which continues up along the [0001] growth direction. The closed dislocations have a 1/3 11-20 edge dislocation Burgers vector component, consistent with known threading dislocations. The open core dislocations are hexagonal shaped with pure screw character, {10-10} side facets, varying lateral widths, and varying degrees of hexagonal symmetry. STEM electron energy loss spectroscopy spectrum imaging revealed a larger C concentration inside the void and below the void than above the void. We propose that carbon deposition during metal organic chemical vapor deposition growth acts as a mask, stopping the GaN deposition locally. Subsequent layers of GaN deposited around the C covered region create the overhanging {10-11} facets, and the meeting of the six {10-11} facets at the pyramid's peak is not perfect, resulting in a dislocation.